An example of a Li-ion battery
(used on the Nokia 3310 mobile phone)
|Specific energy||(0.36–0.875 MJ/kg)|
|Energy density||(0.90–2.43 MJ/L)|
|Specific power||~250-~340 W/kg|
|Self-discharge rate||8% at 21 °C
15% at 40 °C
31% at 60 °C
|Nominal cell voltage||NMC 3.6 / 3.85 V, LiFePO4 3.2 V|
A lithium-ion battery or Li-ion battery is a type of rechargeable battery in which lithium ions move from the negative electrode to the positive electrode during discharge and back when charging. Li-ion batteries use an intercalated lithium compound as one electrode material, compared to the metallic lithium used in a non-rechargeable lithium battery. The electrolyte, which allows for ionic movement, and the two electrodes are the constituent components of a lithium-ion battery cell.
Lithium-ion batteries are common in home electronics. They are one of the most popular types of rechargeable batteries for portable electronics, with a high energy density, tiny memory effect and low self-discharge. Beyond consumer electronics, LIBs are also growing in popularity for military, battery electric vehicle and aerospace applications. For example, lithium-ion batteries are becoming a common replacement for the lead acid batteries that have been used historically for golf carts and utility vehicles. Instead of heavy lead plates and acid electrolyte, the trend is to use lightweight lithium-ion battery packs that can provide the same voltage as lead-acid batteries, so no modification to the vehicle's drive system is required.
Chemistry, performance, cost and safety characteristics vary across LIB types. Handheld electronics mostly use LIBs based on lithium cobalt oxide (LiCoO
2), which offers high energy density, but presents safety risks, especially when damaged. Lithium iron phosphate (LiFePO
4), lithium ion manganese oxide battery (LiMn
3, or LMO) and lithium nickel manganese cobalt oxide (LiNiMnCoO
2 or NMC) offer lower energy density, but longer lives and inherent safety. Such batteries are widely used for electric tools, medical equipment and other roles. NMC in particular is a leading contender for automotive applications. Lithium nickel cobalt aluminum oxide (LiNiCoAlO
2 or NCA) and lithium titanate (Li
12 or LTO) are specialty designs aimed at particular niche roles. The new lithium sulfur batteries promise the highest performance-to-weight ratio.
Lithium-ion batteries can be dangerous under some conditions and can pose a safety hazard since they, unlike other rechargeable batteries, contain a flammable electrolyte and are kept pressurized. Because of this, the testing standards for these batteries are more stringent than those for acid-electrolyte batteries, requiring both a broader range of test conditions and additional battery-specific tests. This is in response to reported accidents and failures, and there have been battery-related recalls by some companies.
Although the word "battery" is a common term to describe an electrochemical storage system, international industry standards differentiate between a "cell" and a "battery". A "cell" is a basic electrochemical unit that contains the basic components, such as electrodes, separator, and electrolyte. In the case of lithium-ion cells, this is the single cylindrical, prismatic or pouch unit, that provides an average potential difference at its terminals of 3.7 V for LiCoO
2 and 3.3 V for LiFePO
4. A "battery" or "battery pack" is a collection of cells or cell assemblies which are ready for use, as it contains an appropriate housing, electrical interconnections, and possibly electronics to control and protect the cells from failure. In this regard, the simplest "battery" is a single cell with perhaps a small electronic circuit for protection.
In many cases, distinguishing between "cell" and "battery" is not important. However, this should be done when dealing with specific applications, for example, battery electric vehicles, where "battery" may indicate a high voltage system of 400 V, and not a single cell. The term "module" is often used as an intermediate topology, with the understanding that a battery pack is made of modules, and modules are composed of individual cells.
Lithium batteries were proposed by M Stanley Whittingham, now at Binghamton University, while working for Exxon in the 1970s. Whittingham used titanium(IV) sulfide and lithium metal as the electrodes. However, this rechargeable lithium battery could never be made practical. Titanium disulfide was a poor choice, since it has to be synthesized under completely sealed conditions. This is extremely expensive (~$1000 per kilo for titanium disulfide raw material in 1970s). When exposed to air, titanium disulfide reacts to form hydrogen sulfide compounds, which have an unpleasant odour. For this, and other reasons, Exxon discontinued development of Whittingham's lithium-titanium disulfide battery. Batteries with metallic lithium electrodes presented safety issues, as lithium is a highly reactive element; it burns in normal atmospheric conditions because of the presence of water and oxygen. As a result, research moved to develop batteries where, instead of metallic lithium, only lithium compounds are present, being capable of accepting and releasing lithium ions.
Reversible intercalation in graphite and intercalation into cathodic oxides was discovered in the 1970s by J. O. Besenhard at TU Munich. Besenhard proposed its application in lithium cells. Electrolyte decomposition and solvent co-intercalation into graphite were severe early drawbacks for battery life.
There were two main trends in the research and development of electrode materials for lithium ion rechargeable batteries. One was the approach from the field of electrochemistry centering on graphite intercalation compounds, and the other was the approach from the field of new nano-carbonaceous materials.
History described above is based on the former stand point. On the other hand, in the recent interview article concerning the first stage of scientific research activity directly related to the LIB developments, it is stated that looking at the major streams in research development, the negative-electrode of today’s lithium ion rechargeable battery has its origins in PAS (polyacenic semiconductive material) discovered by Professor Tokio Yamabe and later Shjzukuni Yata at the beginning of 1980’s. The seed of this technology, furthermore, was the discovery of conductive polymers by Professor Hideki Shirakawa and his group, and it could also be seen as having started from the polyacetylene lithium ion battery developed by MacDiarmid and Heeger et al.
The performance and capacity of lithium-ion batteries increases as development progresses.
Information came to light in 2011 regarding a long-term antitrust violating price-fixing conspiracy among the world's major lithium-ion battery manufacturers that kept prices artificially high from 2000 to 2011, according to a class action complaint that was tentatively settled with one of the defendants, Sony, in 2016. The complaint provided evidence that participants included LG, SD, Sanyo, Panasonic, Sony, and Hitachi, and notes that Sanyo and LG had "pled guilty to the criminal price-fixing of Lithium Ion Batteries."p. Sony agreed to settle for $20 million, and also cooperate by, among other things, making employees chosen by plaintiffs available for interviews, depositions and testimony, as well as provide clarifying information regarding the scheme and the documents provided to date, including responding to authentication and clarification questions. Cooperation clause: page 23 - 25.
The three primary functional components of a lithium-ion battery are the positive and negative electrodes and electrolyte. Generally, the negative electrode of a conventional lithium-ion cell is made from carbon. The positive electrode is a metal oxide, and the electrolyte is a lithium salt in an organic solvent. The electrochemical roles of the electrodes reverse between anode and cathode, depending on the direction of current flow through the cell.
The most commercially popular negative electrode is graphite. The positive electrode is generally one of three materials: a layered oxide (such as lithium cobalt oxide), a polyanion (such as lithium iron phosphate) or a spinel (such as lithium manganese oxide). Recently, graphene based electrodes ( based on 2D and 3D structures of graphene) have also been used as electrodes for lithium batteries. 
The electrolyte is typically a mixture of organic carbonates such as ethylene carbonate or diethyl carbonate containing complexes of lithium ions. These non-aqueous electrolytes generally use non-coordinating anion salts such as lithium hexafluorophosphate (LiPF
6), lithium hexafluoroarsenate monohydrate (LiAsF
6), lithium perchlorate (LiClO
4), lithium tetrafluoroborate (LiBF
4) and lithium triflate (LiCF
Depending on materials choices, the voltage, energy density, life and safety of a lithium-ion battery can change dramatically. Recently, novel architectures using nanotechnology have been employed to improve performance.
Pure lithium is highly reactive. It reacts vigorously with water to form lithium hydroxide and hydrogen gas. Thus, a non-aqueous electrolyte is typically used, and a sealed container rigidly excludes moisture from the battery pack.
Lithium-ion batteries are more expensive than NiCd batteries but operate over a wider temperature range with higher energy densities. They require a protective circuit to limit peak voltage.
For notebooks or laptops, lithium-ion cells are supplied as part of a battery pack with temperature sensors, voltage converter/regulator circuit, voltage tap, battery charge state monitor and the main connector. These components monitor the state of charge and current in and out of each cell, capacities of each individual cell (drastic change can lead to reverse polarities which is dangerous), temperature of each cell and minimize the risk of short circuits.
Cells with a cylindrical shape are made in a characteristic "swiss roll" manner (known as a "jelly roll" in the US), which means it is a single long sandwich of positive electrode, separator, negative electrode and separator rolled into a single spool. The main disadvantage of this method of construction is that the cell will have a higher series inductance.[dubious ]
The absence of a case gives pouch cells the highest gravimetric energy density; however, for many practical applications they still require an external means of containment to prevent expansion when their state-of-charge (SOC) level is high, and for general structural stability of the battery pack of which they are part.
The participants in the electrochemical reactions in a lithium-ion battery are the negative and positive electrodes with the electrolyte providing a conductive medium for lithium ions to move between the electrodes.
Both electrodes allow lithium ions to move in and out of their interiors. During insertion (or intercalation) ions move into the electrode. During the reverse process, extraction (or deintercalation), ions move back out. When a lithium-ion based cell is discharging, the positive lithium ion moves from the negative electrode (usually graphite = "" below) and enters the positive electrode (lithium containing compound). When the cell is charging, the reverse occurs.
The anode (marked -) half reaction is:
In a lithium-ion battery the lithium ions are transported to and from the positive or negative electrodes by oxidizing the transition metal, cobalt (Co), in Li
2 from Co3+
during charge, and reduced from Co4+
during discharge. The cobalt electrode reaction is only reversible for x < 0.5, limiting the depth of discharge allowable. This chemistry was used in the Li-ion cells developed by Sony in 1990.
The cell's energy is equal to the voltage times the charge. Each gram of lithium represents Faraday's constant/6.941 or 13,901 coulombs. At 3 V, this gives 41.7 kJ per gram of lithium, or 11.6 kWh per kg. This is a bit more than the heat of combustion of gasoline, but does not consider the other materials that go into a lithium battery and that make lithium batteries many times heavier per unit of energy.
Liquid electrolytes in lithium-ion batteries consist of lithium salts, such as LiPF
4 or LiClO
4 in an organic solvent, such as ethylene carbonate, dimethyl carbonate, and diethyl carbonate. A liquid electrolyte acts as a conductive pathway for the movement of cations passing from the positive to the negative electrodes during discharge. Typical conductivities of liquid electrolyte at room temperature (20 °C (68 °F)) are in the range of 10 mS/cm, increasing by approximately 30–40% at 40 °C (104 °F) and decreasing slightly at 0 °C (32 °F).
The combination of linear and cyclic carbonates (e.g., ethylene carbonate (EC) and dimethyl carbonate (DMC)) offers high conductivity and SEI-forming ability. A mixture of a high ionic conductivity and low viscosity carbonate solvents is needed, because the two properties are mutually exclusive in a single material.
Organic solvents easily decompose on the negative electrodes during charge. When appropriate organic solvents are used as the electrolyte, the solvent decomposes on initial charging and forms a solid layer called the solid electrolyte interphase (SEI), which is electrically insulating yet provides significant ionic conductivity. The interphase prevents further decomposition of the electrolyte after the second charge. For example, ethylene carbonate is decomposed at a relatively high voltage, 0.7 V vs. lithium, and forms a dense and stable interface.
Composite electrolytes based on POE (poly(oxyethylene)) provide a relatively stable interface. It can be either solid (high molecular weight) and be applied in dry Li-polymer cells, or liquid (low molecular weight) and be applied in regular Li-ion cells.
During charging, an external electrical power source (the charging circuit) applies an over-voltage (a higher voltage than the battery produces, of the same polarity), forcing a charging current to flow within the battery from the positive to the negative electrode, i.e. in the reverse direction of a discharge current under normal conditions. The lithium ions then migrate from the positive to the negative electrode, where they become embedded in the porous electrode material in a process known as intercalation.
The charging procedures for single Li-ion cells, and complete Li-ion batteries, are slightly different.
During the constant current phase, the charger applies a constant current to the battery at a steadily increasing voltage, until the voltage limit per cell is reached.
During the balance phase, the charger reduces the charging current (or cycles the charging on and off to reduce the average current) while the state of charge of individual cells is brought to the same level by a balancing circuit, until the battery is balanced. Some fast chargers skip this stage. Some chargers accomplish the balance by charging each cell independently.
During the constant voltage phase, the charger applies a voltage equal to the maximum cell voltage times the number of cells in series to the battery, as the current gradually declines towards 0, until the current is below a set threshold of about 3% of initial constant charge current.
Periodic topping charge about once per 500 hours. Top charging is recommended to be initiated when voltage goes below 4.05 V/cell.
Failure to follow current and voltage limitations can result in an explosion.
Charging temperature limits for Li-ion are stricter than the operating limits. Lithium-ion chemistry performs well at elevated temperatures but prolonged exposure to heat reduces battery life.
Li‑ion batteries offer good charging performance at cooler temperatures and may even allow 'fast-charging' within a temperature range of 5 to 45 °C (41 to 113 °F).[better source needed] Charging should be performed within this temperature range. At temperatures from 0 to 5 °C charging is possible, but the charge current should be reduced. During a low-temperature charge the slight temperature rise above ambient due to the internal cell resistance is beneficial. High temperatures during charging may lead to battery degradation and charging at temperatures above 45 °C will degrade battery performance, whereas at lower temperatures the internal resistance of the battery may increase, resulting in slower charging and thus longer charging times.[better source needed]
Consumer-grade lithium-ion batteries should not be charged at temperatures below 0 °C (32 °F). Although a battery pack may appear to be charging normally, electroplating of metallic lithium can occur at the negative electrode during a subfreezing charge, and may not be removable even by repeated cycling. Most devices equipped with Li-ion batteries do not allow charging outside of 0–45 °C for safety reasons, except for mobile phones that may allow some degree of charging when they detect an emergency call in progress.
Industry produced about 660 million cylindrical lithium-ion cells in 2012; the 18650 size is by far the most popular for cylindrical cells. If Tesla meets its goal of shipping 40,000 Model S electric cars in 2014 and if the 85-kWh battery, which uses 7,104 of these cells, proves as popular overseas as it was in the U.S., in 2014 the Model S alone would use almost 40 percent of global cylindrical battery production. Production is gradually shifting to higher-capacity 3,000+ mAh cells. Annual flat polymer cell demand was expected to exceed 700 million in 2013.
In 2015 cost estimates ranged from $300–500/kwh.
Because lithium-ion batteries can have a variety of positive and negative electrode materials, the energy density and voltage vary accordingly.
The open circuit voltage is higher than aqueous batteries (such as lead acid, nickel-metal hydride and nickel-cadmium). Internal resistance increases with both cycling and age. Rising internal resistance causes the voltage at the terminals to drop under load, which reduces the maximum current draw. Eventually increasing resistance means that the battery can no longer operate for an adequate period.
Batteries with a lithium iron phosphate positive and graphite negative electrodes have a nominal open-circuit voltage of 3.2 V and a typical charging voltage of 3.6 V. Lithium nickel manganese cobalt (NMC) oxide positives with graphite negatives have a 3.7 V nominal voltage with a 4.2 V maximum while charging. The charging procedure is performed at constant voltage with current-limiting circuitry (i.e., charging with constant current until a voltage of 4.2 V is reached in the cell and continuing with a constant voltage applied until the current drops close to zero). Typically, the charge is terminated at 3% of the initial charge current. In the past, lithium-ion batteries could not be fast-charged and needed at least two hours to fully charge. Current-generation cells can be fully charged in 45 minutes or less. In 2015 researchers demonstrated a small 600 mAh capacity battery charged to 68 percent capacity in two minutes and a 3,000 mAh battery charged to 48 percent capacity in five minutes. The latter battery has an energy density of 620 Wh/L. The device employed heteroatoms bonded to graphite molecules in the anode.
Performance of manufactured batteries has improved over time. For example, from 1991 to 2005 the energy capacity per price of lithium ion batteries improved more than ten-fold, from 0.3Wh per dollar to over 3Wh per dollar.
The increasing demand for batteries has led vendors and academics to focus on improving the energy density, operating temperature, safety, durability, charging time, output power, and cost of lithium ion battery technology. The following materials have been used in commercially available cells. Research into other materials continues.
Cathode materials are generally constructed out of two general materials: LiCoO
2 and LiMn
4. The cobalt-based material develops a pseudo tetrahedral structure that allows for two-dimensional lithium ion diffusion. The cobalt-based cathodes are ideal due to their high theoretical specific heat capacity, high volumetric capacity, low self-discharge, high discharge voltage, and good cycling performance. Limitations include the high cost of the material, slight toxicity, and low thermal stability. The manganese-based materials adopt a cubic crystal lattice system, which allows for three-dimensional lithium ion diffusion. Manganese cathodes are attractive because manganese is cheaper and less toxic than other materials used. Limitations include the tendency for manganese to dissolve into the electrolyte during cycling leading to poor cycling stability for the cathode. Cobalt-based cathodes are the most common however other materials are beginning to be developed to make cheaper and less toxic cathodes.
|Lithium Nickel Manganese Cobalt Oxide ("NMC", LiNixMnyCozO2)||Imara Corporation, Nissan Motor, Microvast Inc.||2008||density, output.|
|Lithium Manganese Oxide ("LMO", LiMn2O4)||LG Chem, NEC, Samsung, Hitachi, Nissan/AESC, EnerDel||Hybrid electric vehicle, cell phone, laptop||1996||durability, cost|
|Lithium Iron Phosphate ("LFP", LiFePO4)||University of Texas/Hydro-Québec, Phostech Lithium Inc., Valence Technology, A123Systems/MIT||Segway Personal Transporter, power tools, aviation products, automotive hybrid systems, PHEV conversions||1996||moderate density (2 A·h outputs 70 amperes) High safety compared to Cobalt / Manganese systems. Operating temperature >60 °C (140 °F)|
Anode materials are generally constructed from graphite and other carbon materials. These materials are used because they are abundant and are electrically conducting and can swell modestly to accommodate the lithium ions associated with building charge. Silicon is beginning to be looked at as an anode material because it can swell much more than graphite, storing up to 10 times more lithium ions, however this swelling can break the electrical contacts in the anode causing catastrophic failure for the battery.
|Graphite||The dominant negative electrode material used in lithium ion batteries.||1991||Low cost and good energy density. Graphite anodes can accommodate one lithium atom for every six carbon atoms. Charging rate is governed by the shape of the long, thin graphene sheets. While charging, the lithium ions must travel to the outer edges of the graphene sheet before coming to rest (intercalating) between the sheets. The circuitous route takes so long that they encounter congestion around those edges.|
|Lithium Titanate ("LTO", Li4Ti5O12)||9,000||Toshiba, Altairnano||automotive (Phoenix Motorcars), electrical grid (PJM Interconnection Regional Transmission Organization control area, United States Department of Defense), bus (Proterra)||2008||output, charging time, durability (safety, operating temperature −50–70 °C (−58–158 °F))|
|Hard Carbon||Energ2||Home electronics||2013||greater storage capacity|
|Tin/Cobalt Alloy||Sony||Consumer electronics (Sony Nexelion battery)||2005||Larger capacity than a cell with graphite (3.5Ah 18650-type battery)|
|Silicon/Carbon||Volumetric: 580 W·h/l||Amprius||Smartphones, providing 5000 mA·h capacity||2013||Uses < 10wt% Silicon nanowires combined with graphite and binders. Energy density: ~74 mAh/g.|
The ions in the electrolyte diffuse because there are small changes in the electrolyte concentration. Linear diffusion is only considered here. The change in concentration, c, as a function of time t and distance x, is
The negative sign indicates the ions are flowing from high concentration to low concentration. In this equation, D is the diffusion coefficient for the lithium ion. It has a value of 7.5 × 10−10 m/s in the LiPF
6 electrolyte. The value for ε, the porosity of the electrolyte, is 0.724.
Li-ion batteries provide lightweight, high energy density power sources for a variety of devices. To power larger devices, such as electric cars, connecting many small batteries in a parallel circuit is more effective and more efficient than connecting a single large battery. Such devices include:
Li-ion batteries are used in telecommunications applications. Secondary non-aqueous lithium batteries provide reliable backup power to load equipment located in a network environment of a typical telecommunications service provider. Li-ion batteries compliant with specific technical criteria are recommended for deployment in the Outside Plant (OSP) at locations such as Controlled Environmental Vaults (CEVs), Electronic Equipment Enclosures (EEEs), and huts, and in uncontrolled structures such as cabinets. In such applications, li-ion battery users require detailed, battery-specific hazardous material information, plus appropriate fire-fighting procedures, to meet regulatory requirements and to protect employees and surrounding equipment.
Batteries gradually self-discharge even if not connected and delivering current. Li+ rechargeable batteries have a self-discharge rate typically stated by manufacturers to be 1.5-2% per month. The rate increases with temperature and state of charge. A 2004 study found that for most cycling conditions self-discharge was primarily time-dependent; however, after several months of stand on open circuit or float charge, state-of-charge dependent losses became significant. The self-discharge rate did not increase monotonically with state-of-charge, but dropped somewhat at intermediate states of charge. Self-discharge rates may increase as batteries age.
For comparison, the self-discharge rate is over 30% per month for common nickel metal hydride (NiMH) batteries, dropping to about 1.25% per month for low self-discharge NiMH batteries, and 10% per month in nickel-cadmium batteries.
Rechargeable battery life is typically defined as the number of full charge-discharge cycles before significant capacity loss. Storage also reduces capacity.
Manufacturers' information typically specify lifespan in terms of the number of cycles (e.g., capacity dropping linearly to 80% over 500 cycles), with no mention of chronological age. Research rejects this common industry practice. On average, lifetimes consist of 1000 cycles, although battery performance is rarely specified for more than 500 cycles. This means that batteries of mobile phones, or other hand-held devices in daily use, are not expected to last longer than three years. Some batteries based on carbon anodes offer more than 10,000 cycles.
As a battery self-discharges, its voltage gradually diminishes. When depleted below the protection circuit's low-voltage threshold (2.4 to 2.9 V/cell, depending on chemistry) the circuit disconnects and stops discharging until recharged. As discharge progresses, metallic cell contents plate onto its internal structure, creating an unwanted discharge path.
A 2015 study by Andreas Gutsch of the Karlsruhe Institute of Technology found that lithium-ion battery storage lifetime could vary by a factor of five, with some Li-ion cells losing 30% of their capacity after 1,000 cycles, and others having better capacity after 5,000 cycles. The study also found that safety standards for some batteries were not met. For stationary energy storage it was estimated that batteries with lifespans of at least 3,000 cycles were needed for profitable operation.
Over their lifespan, batteries degrade progressively with reduced capacity, cycle life, and safety due to chemical changes to the electrodes. Capacity loss/fade is expressed as a percentage of initial capacity after a number of cycles (e.g., 30% loss after 1,000 cycles). Fade can be separated into calendar loss and cycling loss. Calendar loss results from the passage of time and is measured from the maximum state of charge. Cycling loss is due to usage and depends on both the maximum state of charge and the depth of discharge.
Degradation is strongly temperature-dependent; increasing if stored or used at higher temperatures. High charge levels and elevated temperatures (whether from charging or ambient air) hasten capacity loss. Carbon anodes generate heat when in use. Batteries may be refrigerated to reduce temperature effects.
Pouch and cylindrical cell temperatures depend linearly on the discharge current. Poor internal ventilation may increase temperatures. Loss rates vary by temperature: 6% loss at 0 °C (32 °F), 20% at 25 °C (77 °F), and 35% at 40 °C (104 °F). In contrast, the calendar life of LiFePO
4 cells is not affected by high charge states.
The advent of the SEI layer improved performance, but increased vulnerability to thermal degradation. The layer is composed of electrolyte – carbonate reduction products that serve both as an ionic conductor and electronic insulator. It forms on both the anode and cathode and determines many performance parameters. Under typical conditions, such as room temperature and the absence of charge effects and contaminants, after the first charge the layer reaches a fixed thickness, allowing the device can operate for years. However, operation outside such parameters can degrade the device via several reactions.
Five common exothermic degradation reactions can occur:
The SEI layer that forms on the anode is a mixture of lithium oxide, lithium fluoride and semicarbonates (e.g., lithium alkyl carbonates).
At elevated temperatures, alkyl carbonates on the electrolyte decompose into insoluble Li
3 that can increase film thickness, clogging carbon surface pores and limiting ion anode access. This increases impedance and reduces capacity. Gases formed by electrolyte decomposition increase the cell's internal pressure and are a potential safety issue in demanding environments such as mobile devices.
Extended storage can trigger an incremental increase in film thickness and capacity fade.
Charging at greater than 4.2 V can initiate Li+ plating on the anode, producing irreversible capacity fade. The randomness of the metallic lithium embedded in the anode during intercalation results in dendrites formation. Over time the dendrites can accumulate and pierce the separator, causing a short circuit leading to heat, fire and/or explosion. This process is referred to as thermal runaway.
Discharging beyond 2 V can also result in capacity fade. The (copper) anode current collector can dissolve into the electrolyte. When charged, copper ions can reduce on the anode as metallic copper. Over time, copper dendrites can form and cause a short in the same manner as lithium.
In 2016 it was revealed via Wikileaks and other sources that a 4900mAh LiCoO2 cell was being used in military equipment, which overcomes the Cu dendrite issue by substituting gold (Au) as the anode and a classified alloy for the aluminium (needed for high current) cathode current collectors. Other improvements included the use of internal pressure sensors based on MEMS, electrolyte filtering and liquid cooling of the assemblies using SF6.
High cycling rates and state of charge induces mechanical strain on the anode's graphite lattice. Mechanical strain caused by intercalation and de-intercalation creates fissures and splits of the graphite particles, changing their orientation. This orientation change results in capacity fade.
There is a historical note about the terminology of anode when referring to lithium cells, which started as primary (single discharge) as exemplified by lithium thionyl chloride cells. The anode is classically the electrode where oxidation is taking place in electrochemistry. This is true on discharge, but with a rechargeable system the electrode switches back and forth from anode to cathode with cycling. The less ambiguous term for secondary cells electrodes are positive (anode on charge, not discharge) and negative. This is the polarity measured on any cell with a volt meter.
Electrolyte degradation mechanisms include hydrolysis and thermal decomposition.
At concentrations as low as 10 ppm, water begins catalyzing a host of degradation products that can affect the electrolyte, anode and cathode. LiPF
6 participates in an equilibrium reaction with LiF and PF
5. Under typical conditions, the equilibrium lies far to the left. However the presence of water generates substantial LiF, an insoluble, electronically insulating product. LiF binds to the anode surface, increasing film thickness.
6 hydrolysis yields PF
5, a strong Lewis acid that reacts with electron-rich species, such as water. PF
5 reacts with water to form hydrofluoric acid (HF) and phosphorus oxyfluoride. Phosphorus oxyfluoride in turn reacts to form additional HF and difluorohydroxy phosphoric acid. HF converts the rigid SEI film into a fragile one. On the cathode, the carbonate solvent can then diffuse onto the cathode oxide over time, releasing heat and thermal runaway.
Decomposition of electrolyte salts and interactions between the salts and solvent start at as low as 70 C. Significant decomposition occurs at higher temperatures. At 85 C transesterification products, such as dimethyl-2,5-dioxahexane carboxylate (DMDOHC) are formed from EC reacting with DMC.
Lithium cobalt oxide (LiCoO
2) is the most widely used cathode material. Lithium manganese oxide (LiMn2O
4) is a potential alternative because of its low cost and ease of preparation, but its relatively poor cycling and storage capabilities has prevented it from commercial acceptance.
Cathode degradation mechanisms include manganese dissolution, electrolyte oxidation and structural disorder.
4 hydrofluoric acid catalyzes the loss of metallic manganese through disproportionation of trivalent manganese:
2Mn3+ → Mn2++ Mn4+
Material loss of the spinel results in capacity fade. Temperatures as low as 50 C initiate Mn2+ deposition on the anode as metallic manganese with the same effects as lithium and copper plating. Cycling over the theoretical max and min voltage plateaus destroys the crystal lattice via Jahn-Teller distortion, which occurs when Mn4+ is reduced to Mn3+ during discharge.
Storage of a battery charged to greater than 3.6 V initiates electrolyte oxidation by the cathode and induces SEI layer formation on the cathode. As with the anode, excessive SEI formation forms an insulator resulting in capacity fade and uneven current distribution.
Storage at less than 2 V results in the slow degradation of LiCoO
2 and LiMn
4 cathodes, the release of oxygen and irreversible capacity loss.
The need to "condition" NiCd and NiMH batteries has leaked into folklore surrounding Li-ion batteries. The recommendation for the older technologies is to leave the device plugged in for seven or eight hours, even if fully charged. This may be a confusion of battery software calibration instructions with the "conditioning" instructions for NiCd and NiMH batteries.
Li-ion batteries require a battery management system to prevent operation outside each cell's safe operating area (max-charge, min-charge, safe temperature range) and to balance cells to eliminate state of charge mismatches. This significantly improves battery efficiency and increases capacity. As the number of cells and load currents increase, the potential for mismatch increases. The two kinds of mismatch are state-of-charge (SOC) and capacity/energy ("C/E"). Though SOC is more common, each problem limits pack charge capacity (mA·h) to that of the weakest cell.
If overheated or overcharged, Li-ion batteries may suffer thermal runaway and cell rupture. In extreme cases this can lead to combustion. To reduce these risks, lithium-ion battery packs contain fail-safe circuitry that disconnects the battery when its voltage is outside the safe range of 3–4.2 V per cell. Lithium-ion cells are very susceptible to damage outside the allowed voltage range that is typically within (2.5 to 3.65) V for most LFP cells. Exceeding this voltage range results in premature aging of the cells and, furthermore, results in safety risks due to the reactive components in the cells. When stored for long periods the small current draw of the protection circuitry may drain the battery below its shutoff voltage; normal chargers may then be useless. Many types of lithium-ion cells cannot be charged safely below 0 °C.
Other safety features are required in each cell:
These devices occupy useful space inside the cells, add additional points of failure and irreversibly disable the cell when activated. They are required because the negative electrode produces heat during use, while the positive electrode may produce oxygen. These devices and improved electrode designs reduce/eliminate the risk of fire or explosion. Further, these features increase costs compared to nickel metal hydride batteries, which require only a hydrogen/oxygen recombination device (preventing damage due to mild overcharging) and a back-up pressure valve. Contaminants inside the cells can defeat these safety devices. These features can not be applied to all kinds of cells. Prismatic high current rate cells can not be equipped with vent or thermal interrupt. This type of modern cells need to do the job even if they short circuit for couple of seconds. This conditions may happen in some cases such as capacitors rush current or even repairman faulty limited short circuits. High current cells (may by up to 30 C, SLPB11543140H5 ) must not produce any excessive heat or oxygen. Instead they must be equipped with newly designed internal thermal fuses which act before the anode and cathode reaches their thermal runaway limits. As this type of fuses integrated internally safety code NAVSEA9310 accepted them in their test procedure.[clarification needed]
Short-circuiting a battery will cause the cell to overheat and possibly to catch fire. Adjacent cells may then overheat and fail, possibly causing the entire battery to ignite or rupture. In the event of a fire, the device may emit dense irritating smoke. The fire energy content (electrical + chemical) of cobalt-oxide cells is about 100 to 150 kJ/(A·h), most of it chemical.
Replacing the lithium cobalt oxide positive electrode material in lithium-ion batteries with a lithium metal phosphate such as lithium iron phosphate improves cycle counts, shelf life and safety, but lowers capacity. As of 2006 these 'safer' lithium-ion batteries were mainly used in electric cars and other large-capacity battery applications, where safety is critical.
Lithium-ion batteries, unlike other rechargeable batteries, have a potentially hazardous pressurised flammable electrolyte, and require strict quality control during manufacture. A faulty battery can cause a serious fire. Faulty chargers can affect the safety of the battery because they can destroy the battery's protection circuit. While charging at temperatures below 0 °C, the negative electrode of the cells gets plated with pure lithium, which can compromise the safety of the whole pack.
While fire is often serious, it may be catastrophically so. In about 2010 large lithium-ion batteries were introduced in place of other chemistries to power systems on some aircraft; as of January 2014[update] there had been at least four serious lithium-ion battery fires, or smoke, on the Boeing 787 passenger aircraft, introduced in 2011, which did not cause crashes but had the potential to do so.
In addition, several aircraft crashes have been attributed to burning Li-Ion batteries. UPS Flight 6 crashed in Dubai after its payload of batteries spontaneously ignited, progressively destroying critical systems inside the aircraft which eventually rendered it uncontrollable.
Since Li-ion batteries contain less toxic metals than other types of batteries which may contain lead or cadmium they are generally categorized as non-hazardous waste. Li-ion battery elements including iron, copper, nickel and cobalt are considered safe for incinerators and landfills. These metals can be recycled, but mining generally remains cheaper than recycling. At present, not much is invested into recycling Li-ion batteries due to costs, complexities and low yield. The most expensive metal involved in the construction of the cell is cobalt. Lithium iron phosphate is cheaper but has other drawbacks. Lithium is less expensive than other metals used, but recycling could prevent a future shortage. The manufacturing processes of nickel and cobalt for the positive electrode and also the solvent, present potential environmental and health hazards. Manufacturing a kg of LiOn battery takes energy equivalent to 1.6 kg of oil.
In December 2005 Dell recalled approximately 22,000 laptop computer batteries, and 4.1 million in August 2006. Approximately 10 million Sony batteries used in Dell, Sony, Apple, Lenovo, Panasonic, Toshiba, Hitachi, Fujitsu and Sharp laptops were recalled in 2006. The batteries were found to be susceptible to internal contamination by metal particles during manufacture. Under some circumstances, these particles could pierce the separator, causing a dangerous short-circuit.
In March 2007 computer manufacturer Lenovo recalled approximately 205,000 batteries at risk of explosion. In August 2007 mobile phone manufacturer Nokia recalled over 46 million batteries at risk of overheating and exploding. One such incident occurred in the Philippines involving a Nokia N91, which used the BL-5C battery.
In September 2016 Samsung recalled approximately 2.5 million Galaxy Note 7 phones after 35 confirmed fires. The recall was due to a manufacturing fault in Samsung's batteries which cause the positive and negative poles to come into contact.
The maximum size of each battery (whether installed in a device or as spare batteries) that can be carried is one that has an equivalent lithium content (ELC) not exceeding 8 grammes per battery. Except, that if only one or two batteries are carried, each may have an ELC of not more than 25 grammes each. The ELC for any battery is found by multiplying the ampere-hour capacity of each cell by 0.3 and then multiplying the result by the number of cells in the battery. The resultant calculated lithium content is not the actual lithium content but a theoretical figure solely for transportation purposes. When shipping lithium ion batteries however, if the total lithium content in the cell exceeds 1.5 g, the package must be marked as "Class 9 miscellaneous hazardous material".
Although devices containing lithium-ion batteries may be transported in checked baggage, spare batteries may be only transported in carry-on baggage. They must be protected against short circuiting, and example tips are provided in the transport regulations on safe packaging and carriage; e.g., such batteries should be in their original protective packaging or, "by taping over the exposed terminals or placing each battery in a separate plastic bag or protective pouch". These restriction do not apply to a lithium-ion battery that is a part of a wheelchair or mobility aid (including any spare batteries) to which a separate set of rules and regulations apply.
Some postal administrations restrict air shipping (including EMS) of lithium and lithium-ion batteries, either separately or installed in equipment. Such restrictions apply in Hong Kong, Australia and Japan.
On 16 May 2012, the United States Postal Service (USPS) banned shipping anything containing a lithium battery to an overseas address, after fires from transport of batteries. This restriction made it difficult to send anything containing lithium batteries to military personnel overseas, as the USPS was the only method of shipment to these addresses; the ban was lifted on 15 November 2012. United Airlines and Delta Air Lines excluded lithium-ion batteries in 2015 after an FAA report on chain reactions.
Researchers are working to improve the research methods, power density, safety, cycle durability, recharge time, cost, flexibility, and other characteristics of these batteries. Researchers at IBM India have come up with an experimental power supply using lithium-ion cells from discarded laptop battery packs for use in unelectrified regions in developing nations.
|Wikimedia Commons has media related to Lithium-ion batteries.|